Understanding Fatigue Analysis
This document provides background information on fatigue and describes the methodology used
in Pro/MECHANICA fatigue analysis. It covers the following topics:
• History of Fatigue
• Physics of Fatigue
• The E-N Approach
Includes the effect of mean residual stresses, hysteresis loop capture and rainflow
Factors that Affect Fatigue Life
Includes Component Size, Loading Type, Surface Finish, Surface Treatment (i.e.
Mechanical Treatments, Plating, and Thermal Treatments), and Effect of Surface
Treatments on Endurance Limit.
The solver technology integrated with Pro/MECHANICA fatigue analysis is provided by nCode,
Inc. Fatigue analysis requires a Fatigue Advisor license from PTC.
History of Fatigue
The majority of component designs involve parts subjected to fluctuating or cyclic loads. Such
loading induces fluctuating or cyclic stresses that often result in failure by fatigue. About 95% of
all structural failures occur through a fatigue mechanism.
The damage done during the fatigue process is cumulative and generally unrecoverable, due to
• It is nearly impossible to detect any progressive changes in material behavior during the
fatigue process, so failures often occur without warning.
• Periods of rest, with the fatigue stress removed, do not lead to any measurable healing or
It was well-known that wood or metal could be made to break by repeatedly bending it back and
forth with a large amplitude. But, it was then discovered that repeated stressing can produce
fracture even when the stress amplitude is apparently well within the elastic range of the material.
When fatigue failures of railway axles became a widespread problem in the middle of the
nineteenth century, this drew attention to cyclic loading effects. This was the first time that many
similar components had been subjected to millions of cycles at stress levels well below the
monotonic tensile yield stress. Between 1852 and 1870 the German railway engineer August
Wöhler set up and conducted the first systematic fatigue investigation.
Some of Wöhler's data are for Krupp axle steel and are plotted, in terms of nominal stress (S) vs.
number of cycles to failure (N), on what has become known as the S-N diagram. Each curve on
such a diagram is still referred to as a Wöhler line.
(Steel supplied in 1862)
(Steel supplied in 1862)
(Steel supplied in 1853)
(Steel supplied in 1853)
Note: 1centner = 50 kg, 1 zoll = 1 inch, 1 centner/zoll2 ~ 0.75 MPa
At about the same time, other engineers began to concern themselves with problems of failures
associated with fluctuating loads in bridges, marine equipment, and power generation machines.
During the first part of the twentieth century, more effort was placed on understanding the
mechanisms of the fatigue process rather than just observing its results. This activity finally led,
in the late fifties and early sixties, to the development of the two approaches, one based on linear
elastic fracture mechanics, LEFM, to explain how cracks propagate, and the so-called CoffinManson local strain methodology to explain crack initiation. Through this understanding, modern
designers and engineers have been able to create more fatigue resistant components without
relying solely on experimentation. From a practical point of view, this has been a much more
Physics of Fatigue
Since 1830, it has been recognized that metal under a repetitive or fluctuating load will fail at a
stress level lower than required to cause failure under a single application of the same load.
The following diagram shows a simple component subjected to a uniform sinusoidally varying
force. After a period of time, a crack can be seen to initiate on the circumference of the hole.
This crack will then propagate through the component until the remaining intact section is
incapable of sustaining the imposed stresses and the component fails.
Stress range, Sr
The physical development of a crack is generally divided into 2 separate stages. These relate to
the crack initiation phase (Stage I) and the crack growth phase (Stage II). Fatigue cracks initiate
through the release of shear strain energy. The following diagram shows how the shear stresses
result in local plastic deformation along slip planes. As the loading is cycled sinusoidally, the slip
planes move back and forth like a pack of cards, resulting in small extrusions and intrusions on
the crystal surface. These surface disturbances are approximately 1 to 10 microns in height and
constitute embryonic cracks.
Slip bands form
along planes of
giving rise to
A crack initiates in this way until it reaches the grain boundary. At this point the mechanism is
gradually transferred to the adjacent grain
When the crack has grown through approximately 3 grains, it is seen to change its direction of
propagation. Stage I growth follows the direction of the maximum shear plane, or 45° to the
direction of loading. During Stage II the physical mechanism for fatigue changes. The crack is
now sufficiently large to form a geometrical stress concentration. A tensile plastic zone is created
at the crack tip as shown in the following diagram. After this stage, the crack propagates
perpendicular to the direction of the applied load.
Crack showing stress
concentration at the tip
As the physical mechanism for fatigue is divided into two stages, the methods of analysis are also
conventionally divided into two stages. Stage I is typically analyzed using the local strain (or E-N)
approach, while Stage II is analyzed using a fracture mechanics based approach.
A complete fatigue prediction could therefore use a combination of both methods:
Total Life = Life to initiation + Life taken to propagate crack to failure
However, most engineering components spend most of their time at either one stage or the other.
In this case, it is normal to conservatively consider only one stage. For example, in most ground
vehicle designs, life is typically governed by time to initiation. Components are relatively stiff and
the materials fairly brittle. Once the crack has initiated, it takes a relatively short time to
propagate to failure.
By contrast, many aerospace applications use flexible components made of very ductile
materials. In this case, cracks propagate relatively slowly and so the fracture mechanics
approaches are usually more appropriate.
The physical nature of fatigue was not widely understood during the early days. August Wöhler
therefore took a more pragmatic view of fatigue analysis. The method he developed later
became known as nominal stress (or S-N) fatigue analysis. This did not differentiate between the
Stage I and II growth methods and instead related the nominal stress range to the time taken to
Though S-N analysis is still widely used in test based fatigue analysis, it has one major drawback
for CAE applications. Fatigue initiation is driven by local plastic strains, but S-N analysis uses
elastic stress as the input. Therefore, S-N analysis is unsuitable for performing CAE analysis on
components containing local areas of plasticity. For this reason local strain (or E-N) methods are
more universally suitable. This product uses the E-N method.
The E-N Approach
In a fatigue test, hourglass-shaped specimens of different material types are subjected to various
types of cyclic loading, such as: small-scale bending, torsion, tension, and compression. The EN approach uses these tests to measure fatigue life. The results are plotted in terms of strain (E)
vs. cycles to failure (N) on an E-N diagram. A typical E-N diagram is illustrated below for a low
alloy steel and an aluminum alloy.
Sf': 975 b: -0.087 Ef': 0.583 c: -0.58
Sf': 1086 b: -0.095 Ef': 0.35 c: -0.69
Strain Life Plot
Strain Amplitude (M/M)
Pro/MECHANICA uses a generic set of fatigue properties to model low alloy steels, unalloyed
steels, aluminum alloys, and titanium alloys. These generic properties have been compiled by
Baumel Jr. and Seeger and are known as the Uniform Material Law. While they cannot be
expected to give accurate fatigue lives for practical purposes, they are ideal for determining
whether a component is likely to suffer from fatigue problems, and whether a more detail analysis
is needed before commissioning.
Before looking in more detail at the E-N procedure, it helps to understand the three different types
of cyclic strains that contribute to the fatigue process. The following diagrams and descriptions
explain each separate type.
The first figure illustrates a fully-reversed strain cycle with a sinusoidal form. This is an idealized
loading condition typically found in rotating shafts operating at constant speed without overloads.
This is also the type of strain cycle used for most fatigue tests. For this kind of cycle, the
maximum (εmax) and minimum (εmin) strains are of equal magnitude but opposite sign. Usually
tensile strain is considered to be positive and compressive strain negative. The strain range, εr, is
the algebraic difference between the maximum and minimum strains in a cycle.
εr = εmax − εmin
The strain amplitude, εa, is one half the strain range.
εa = εr / 2 = (εmax − εmin) / 2
- Compressive Tensile +
The second figure illustrates the more general situation where the maximum and minimum strains
are not equal. In this case, they are both tensile and define a mean offset, εm = (εmax + εmin) / 2,
for the cyclic loading.
As mentioned above, most basic fatigue data are collected using fully-reversed loads. Therefore,
these data are not directly applicable for strain cycles with a non-zero mean (εm ≠ 0). In order to
predict more realistic life estimates for strain cycles with tensile or compressive mean stress,
results of the tests conducted using fully-reversed loads are corrected. The choice of corrective
approach to use depends on whether the mean stress is primarily tensile or compressive.
The reason for this can be seen in the following plot which schematically illustrates the effect of
mean stress on the strain-life (E-N) curve. Viewed conceptually, tensile mean stress acts to pull
open a crack while compressive mean stress works to keep it closed. Typically the effects are
concentrated at the long life end of the diagram, with tensile mean stress reducing life and
compressive mean stress extending it.
Log Strain Amplitude
Compressive Mean Stress
Fully Reversed (zero mean stress)
Tensile Mean Stress
Since the tests required to calculate E-N curves for a range of mean stresses are quite
expensive, several empirical relationships have been developed to model the effect of mean
stress. Of all the proposed methods, two have been most widely accepted:
• The Smith, Watson, Topper Approach
• The Morrow Correction
For loading sequences which are predominantly tensile in nature, the Smith, Watson, Topper
approach is more conservative and is therefore recommended. In the case where the loading is
predominantly compressive, particularly for wholly compressive cycles, the Morrow correction can
be used to provide more realistic life estimates. Pro/MECHANICA uses both methods and the
most appropriate method is automatically chosen.
The next figure illustrates a more complex, variable amplitude loading pattern that is closer to the
cyclic strains found in real structures.
For variable amplitude loading it is necessary to extract the fatigue damaging cycles from the
signal and then evaluate the damage carried out by each cycle. The total damage is the sum of
the damage caused by each individual cycle. Each fatigue cycle is extracted by a process known
as hysteresis loop capture. The loci of the stress and strain are plotted as shown in the following
Strain Amplitude = ½ Strain Range
When a stress-strain hysteresis loop is closed, then the strain range and mean stress are
returned and the damage calculated using the E-N curve modified for mean stress correction.
This analysis is carried out over the whole strain time signal until all the cycles have been
extracted and the total damage evaluated. A very efficient algorithm has been developed to
perform cycle extraction known as: Rainflow Cycle Counting. This is the algorithm that
Pro/MECHANICA normally uses a linear elastic solution to determine the pseudo-elastic strains in
a component. In other words, the solution ignores plasticity. Before proceeding with the fatigue
analysis, these strains are automatically converted into non-linear elastic-plastic strains using
Factors that Affect Fatigue Life
As mentioned above, the E-N curve is derived from strain control tests based on hourglassshaped specimens.
A standardized, fully reversed fatigue test is used to determine a base-line E-N relationship for a
polished specimen, approximately 6 mm in diameter. While the fatigue or endurance limit
measured in this test is denoted by ε'e, a component in service has lower limit, εe, that reflects
modifications to a specimen outside of the laboratory. For steels in particular, several empirical
relationships account for the variation in εe as a result of the following:
• Component size, Csize
• The type of loading, Cload
• The effect of notches, Cnotch
• The effect of surface finish, Csur < 1 (promotes crack growth)
• The effect of surface treatment, Csur >1 (inhibits crack growth)
To account for these effects, specific modifying factors are typically applied to the test result so
εe = ε'eCnotchCsizeCloadCsur . . .
where reciprocal of the product, CnotchCsizeCloadCsur , is collectively known as the fatigue strength
reduction factor Kf:
Kf = 1 / (CnotchCsizeCloadCsur . . .)
It is very important to remember that all the modification factors are empirical, conservative and
generally only applicable to steel. They provide little or no fundamental insight into the fatigue
process itself other than providing approximate trends. In particular they should not be used in
areas outside their measured applicability.
The Influence of Component Size
Fatigue in metals results from the nucleation and subsequent growth of crack-like flaws under the
influence of an alternating stress field. The theory is that failure starts at the weakest link, the
most favorably orientated metal crystal for example, and then grows through less favorably
orientated grains until final failure. Intuitively, it would seem reasonable to suppose that the larger
the volume of material subjected to the alternating stress, the higher the probability of finding the
weakest link sooner. Actual test data do confirm the presence of a size effect particularly in the
case of bending and torsion.
The stress gradient built up through the section, in bending and to a lesser extent in torsion,
concentrates more than 95% of the maximum surface stress in a thin layer of surface material. In
large sections, this stress gradient is less steep than in smaller sections. So the volume of
material available that could contain a critical flaw will be greater, leading to a reduced fatigue
strength. The effect is small for axial tension where the stress gradient is absent. The value for
Csize is estimated from one of the following.
If the diameter of the test specimen shaft is d < 6 mm:
Csize = 1
If the diameter of the test specimen shaft is 6 mm < d < 250 mm
Csize = 1.189d-0.097
The effect of size is particularly important for the analysis of rotating shafts such as might be
found in vehicle powertrains.
For situations where components do not have a round cross section, the following equation
calculates an equivalent diameter, deq, for a rectangular section under bending with width (w) and
deq2 = 0.65wt
The Influence of Loading Type
Fatigue data measured using one type of cyclic loading, axial tension for example, may be
corrected" to represent the data that would have been obtained had the test been performed
using some other loading methodology such as torsion or bending. The standardized rotating
bend test calls for tests to be carried out under conditions of fully reversed bending.
In moving from one loading condition to another, the values of Cload to be used with the
endurance limit, εe are detailed below:
Thus, using the values from this table, if an axial tension load produces a strain of εe, the strain
produced under a bending load would be 1.25εe.
In addition to influencing the endurance limit, loading conditions can also influence the Basquin
slope, b, which is used when plotting the E-N curve on log-log scale. This effect is usually taken
into account by modification of the strain at 103 cycles, ε3, as well as εe. The following factors are
used to define C'load, the ε3 modification factor:
The Influence of Surface Finish
A very high proportion of all fatigue failures nucleate at the surface of components so that surface
conditions become an extremely important factor influencing fatigue strength. Various surface
conditions are usually judged against the polished laboratory specimen standard. Normally,
scratches, pits, machining marks, and so forth, influence fatigue strength by providing additional
stress raisers that aid the process of crack nucleation.
The diagram below shows that high strength steels are more adversely affected by a rough
surface finish than softer steels. For this reason, the surface finish correction factor, Csur < 1, is
strongly related to tensile strength. Here the surface finish correction factor categorizes finish in
qualitative terms such as polished, machined, and forged.
Fine Ground/Commercially Polished
Corroded in Tap Water
Corroded in Salt Water
80 100 120 140 160 180 200 220 240 260
Tensile Strength, Su (ksi)
Note that some of the curves presented in this figure include effects other than just surface finish.
For example, the forged and hot rolled curves include the effect of decarburization.
Other diagrams present the surface finish correction factor in a more quantitative way by using a
quantitative measure of surface roughness such as RA (the root mean square) or AA (the
arithmetic average). The following diagram shows the effect of surface roughness on the surface
finish correction factor.
Tensile Strength, Su (ksi)
Values of surface roughness associated with each of the manufacturing processes are readily
available in handbooks, as in the example below:
Type of Finish
Partly hand polished
Ground and polished
The Qualitative Influence of Surface Treatment
As in the case of surface finish, surface treatment can greatly influence fatigue strength,
particularly the endurance limit. The net effect of the treatment is to alter the state of residual
stress at the free surface.
M1 applied at T=1
M2 applied at T=2
No moment applied at T=3
Residual stresses arise when plastic deformation is not uniformly distributed throughout the entire
cross section of the component being deformed. In the preceding figures, a metal bar has a
surface that is being deformed in tension by bending.
• At time T=1, bending moment M1 is being applied and is in the elastic range.
• At time T=2, the bending moment has increased to M2, the yield stress (Sy) has been
reached, and the surface undergoes plastic deformation.
• When the external force is removed, the regions that were plastically deformed prevent the
adjacent elastic regions from complete elastic recovery to the unstrained condition. In this
way, the elastically deformed regions are left in residual tension, and the plastically deformed
regions are in a state of residual compression. The result is the stress distribution at time
For many purposes, residual stress can be considered identical to the stresses produced by an
external force. Thus, the presence of a compressive residual stress at the surface of a
component will effectively decrease the probability of fatigue failure.
+Smax + SR
+Smax + SR
The preceding figure illustrates the superposition of applied and residual stresses.
• The top schematic shows an elastic stress distribution in a beam under bending moment M
with no residual stress.
• In the center schematic, a typical residual stress distribution associated with a mechanical
surface treatment such as shot peening is detailed. Note that the compressive stress at the
surface is compensated by an equivalent tensile stress over the interior of the cross section.
• In the bottom schematic, the distribution due to the algebraic summation of the applied stress
(caused by bending moment M) and residual stress is shown. Note that the maximum tensile
stress at the surface has been reduced by the amount of the residual stress. Also, the peak
tensile stress has now been moved to the interior of the beam. The magnitude of this stress
will depend on the gradient of the applied stress and the residual stress distribution. Under
these conditions, subsurface crack initiation becomes a possibility.
Surface treatments are divided broadly into mechanical, thermal, and plating processes. The first
two processes provide a compressive layer. The plating process provides a tensile residual
stress. Following is detailed description of each process:
• Mechanical Treatments The main commercial methods for introducing residual
compressive stresses are cold rolling and shot peening. Although some alteration in the
strength of the material occurs as a result of work hardening, the improvement in fatigue
strength is due mainly to the compressive surface stress. Surface rolling is particularly suited
to large parts and is frequently used in critical components such as crankshafts and the
bearing surface of railway axles. Bolts with rolled threads typically possess twice the fatigue
strength of conventionally machined threads.
Shot peening, which consists of firing fine steel or cast iron shot against the surface of a
component, is particularly well suited to processing small mass produced parts.
It is important to remember that cold rolling and shot peening have their greatest effect at
long lives. At short lives they have little or no effect.
As with other modifying factors, correction factors can be used to account for the effect of
these mechanically induced compressive stresses by adjusting the endurance limit εe.
Typically the factor associated with peening is about 1.5 to 2.0.
• Thermal Treatments Thermal treatments are processes that rely on the diffusion of either
carbon (carburizing) or nitrogen (nitriding) onto and into the surface of a steel component.
Both types of atoms are interstitial, that is they occupy the spaces between adjacent iron
atoms, thereby increasing the strength of the steel and causing a compressive residual stress
to be left on the surface through volumetric changes.
Carburising is typically a three-step process:
packing the steel components within boxes which contain carbonaceous solids
sealing to exclude the atmosphere
heating to about 900 degrees Celsius for a period of time that depends on the depth
of the case required
Alternatively components may be heated in a furnace in the presence of a hot carburizing gas
such as natural gas. This process has the advantage that it is quicker and more accurate. In
addition, the carburizing cycle may be followed up by a diffusion cycle with no carburizing
agent present. This allows some of the carbon atoms to diffuse further into the component
and thus reduces gradients.
The nitriding process is very similar in nature to gas carburizing except that ammonia gas is
used and the components are soaked at lower temperatures. Typically 48 hours at about
550 degrees Celsius will provide a nitrided case depth of about 0.5 mm. Nitriding is
particularly suited to the treatment of finished notched components such as gears and slotted
shafts. The effectiveness of the process is illustrated in the following table:
Endurance Limit (MPa)
• Plating Chrome and nickel plating of steel components can decrease the endurance limit
by more than half, due to the creation of tensile residual stresses at the surface. These
tensile stresses are a direct result of the plating process itself. As in the case of mechanically
induced surface stresses, the effect of plating is most pronounced at the long life end of the
spectrum and also with higher strength materials.
Introducing a compressive residual stress prior to the plating process such as shot peening or
nitriding can reduce the harmful effects of plating. Annealing components after plating,
thereby relieving the tensions, is an alternative approach.
The Quantitative Effect of Surface Treatments on the Endurance Limit
The effect of surface treatment depends on the surface finish. The increase in endurance limit
stress due to the surface treatment is given in the following table:
Increase in Endurance Limit
Whatever correction was made by the surface finish, applying a surface treatment will have a
subsequent effect based on the preceding table. For example, if machining reduces the
endurance limit by 30%, then from the table it can be seen that cold rolling will recover the loss by
increasing the limit 70%.